IS : 1199- 1959
( Reaffirmed IS91 1
METHODS OF SAMPLING AND
ANALYSIS OF CONCRETE
( Eleventh Reprint NOVEMBER 1991 )
UDC 666’97 : 620’11
0 Copyrfght 1959
BUREAU OF INDIAN STANDARDS
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARO
NEW DELHI 110002
( Reaffirmed 1999 )
METHODS OF SAMPLING AND
ANALYSIS OF CONCRETE
Cement and Concrete Sectional Committee, BDC 2
SHRI E. A. NADIRSHAH The Concrete Association of India, Bombay; wtd
The Institution of Engineers ( India ), Calcutb
SXRIBALEUWAR NATH Central Board of Irrigation & Power (Ministry of
Irrigation 4%Power )
Smu N. H. BHAOWANANI Engineer-in-Chief’s Branch, Army Headquarters
SHRIN. D. DAPTARY Bombay State Road Transport Corporation, Bombay
SHRIP. L. Drs Directorate General of Supplies & Disposals
( Ministfy ?f Works, Housing &.Supply )
Cent;rarfe;ldmg Research Instttute ( CSIR),
SHRI C. H. KHADILKAR( ALtcmute )
SHRI C. L. HANDA Directorate of Designs, Bhakra Dam, New D&i
SHRIP. S. BHATNAOAR( A&mats )
DR R, R. HA~ANOADI The Associated Cement Companies Ltd, Bombay
SRRZV. N. PN (Alternate)
Sm p. C. HAZRA Geological Survey of India, Calcutta
DR R. C. HOON Ccnkal Water & Power Commission ( Ministry of
Irrigation h Power)
SHRI GEOROE O~MWN (A&emote) .
SHRIS. B. Jom S. B. Joshi & Co, Bombay
SHRIS. R. MEHRA Central Road Research Institute ( CSIR ), New D&i
SHRIS. N. MUKERJI Government Test House, Calcut_ta
SHRIK. K. CW-I’IWJeE ( Altemu~)
SWRIE. P. NC~OI+AIDE~ Gammon India Ltd, Bombay; md Indian Roads
Congress, New Delhi
REPRESBVATIVE Martin Burn Ltd, Calcutta
SHRIJ. M. RIJHWANI Central Public Works Department
SHRIM. S. BIiAnA ( Altmate )
SHRINIHAR OIANDRA ROY Dahnia Cement ( Bharat ) Ltd, Calcutta
SHRIA. K. CHAKRAVARTJ(Al&mate )
SHRISARIJPSIh’CIi National Buildings Organisation ( Ministry of Works,
Housing & Supply )
DEPUIY DIRECIQR (MATE-
RIAL ) (Alternate)
( Continuedonpag#2 )
BUREAU OF INDIAN STANDARDS
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARG
NEW DELHI 110002
SHRIK. k SGoD
Sls$u c. s. CssAND-~
RoadsWq, Midry ofTruyport & Commtmica-
Research, Design & Stmhrdizatiou Orgahation
( Ministry of Railwaya )
Deputy Director ( 81dg ), BiS
Concrete Subcommittee, BhZ 2 : 2
SRU S. B. Jostr S. B. Josbi & Co, Bombay
sramK. F. ANTIA The Associated Cement Companies Ltd. Bombay
S~nr N. H. BHAGWANANI Engineer-in-Chief’s Branch, Army Headquartas
SHIUM. s. BHATIA Central Public Worka Department
SW T: S. VEDAGlIu ( dffcfIkat-9)
DZRZCTOR Engineering Research Laboratories, Hyderabad
h$sRP.Cc.H~NB^ Geological Survey of India, Calcutta
. . Central Water & Power Commission ( Miuhtry of
Ilvigatiog h Power )
&mt C. L. N. LY&NGAR The Concrete Association of India, Bombay
Strru S. V. NATU Public Works Department, Bombay
SH~UC. C: PATBL ( Allmrofc)
SB&EEiP.~o~L-~ Gammon Eudia Ltd. Bombay
. . Central.W_ater & Powyr Commission ( Miuistry of
Stim SUP SXNGH
Bmldmga Orgauisation ( Miuistry of Works,
HousinR & SUDPIY1
&mlH.P.SlNnA Roads Wing, Ministry of Transport & Commtica-
BornrK. c.SOoD Research, Dcsigu & Stamhrdhtiou Organization
METHODS OF SAMPLING AND
ANALYSIS OF CONCRETE
0.1 This Indian Standard was adopted by the Indian Standards Institu-
tion on 10 November 1,959, after the draft finalized by tht Cement and
Foz;e Sectional Commtttee had been approved by the B&ding Division
0.2 Testing plays an important role in controlling the quality of cement
concrete work. Systematic testing of the raw materials for concrete as
also, the concrete, both while it is fresh and after it has hardened, is an
inseparable part of any quality control programme for concrete. It helps
to achieve higher efficiency of the materials used and greater assurance of
the performance of the concrete in regard to both strength and durability.
The test methods used should be simple, direct and convenient in their
application. This standard has been prepared with this object in view
and provides a guide to the sampling, analysis, and determination of linear
changes of concrete. Strength tests for concrete have been covered
separately in IS : 516-1959 Methods of Tests for Strength of Concrete.
0.3 The Sectional Committee responsible for the preparation of this stand-
ard has taken into consideration the views of concrete specialists, testing
authorities, consumers and technologists and has related the standard to
the practices followed in the country in this field. The need for inter-
national co-ordination between standards prevailing in different countries
of the world has also been recognized. These considerations led the
Sectional Committee to derive assistance from the published standards and
publications of the following organizations:
RESEARCH,DESIGN & STANDARDIZATIONORGANIZATION,MINISTRY
‘THE CONCRETEA~~OCXATIONOF INDIA
0.4 The Indian Standard Methods of
(IS: 516-1959 ) is a necessary adjunct
Tests for Strength of Concrete
to this standard. Besides, this
IS : 1199- 1959
standard requires reference to the following Indian Standards:
*IS : 269-1958 SPECIFICATIONFOKORDINARY, RAPID-HARDENINGAND
Low HEAT PORTLANDCEMENT( Revised)
ttlS : 383-1952 SPECIFICATIONFOR COARSE AND FINE AGGREGATU
$IS : 460-1953 SPECIFICATIONFORTEST SIEVES
0.4.1 Wherever a reference to any standard mentioned under 0.4, except
JS : 460-1953, appears in this standard, it shall be taken as a reference to
the latest version of the standard.
0.5 In pursuance of the decision of the Government of India to introduce
a uniform system of weights and measures throughout the country based
on the metric system, in this standard all dimensions and values have
‘been given in metric units only. It is hoped that this step will facilitate
the change-over to the metric system by the industry more expeditiously.
0.6 For the purpose of deciding whether a particular requirement of this
standard is complied with, the final value, observed or calculated, express-
ing the result of a test or analysis, shall be rounded off in accordance with
‘;IS : 2-1949 Rules for Rounding Off Numerical Values. The number of
significant places retained in the rounded off value should be the same as
that of the specified value in this standard.
0.7 This standard is intended chiefly to cover the technical provisions
relatiDg to sampling and analysis of concrete, and it does not include all
the fiecessary, provisions of a contract.
1.1 This standard covers the methods of taking samples of concrete and
2.0 For the purpose of this standard, the foilowing definitions shall apply.
2.1 Absorption (Air-Dry Basis ) - The percentage of water absorbed
by an air-dried aggregate when immersed in water at 27°C for a period
of 24 hours.
2.2 Absorption ( Saturated Surface-Dry Basis ) - The percentage
of water absorbed by an aggregate when immersed in water at 27°C
for 24 hours, the aggregate being previously dried in an oven at I05 to
110°C to constant weight.
2.3 Admixture -A material other than water, aggregates and portland
cement used as an ingredient of concrete and added to it immediately
before or during its mixing.
2.4 Air-Entrained Concrete -Concrete Containing a small volume of
air deliberately rntrained in the form of minute discrete air voids by the
addition of an a&entraining agent.
2.3 Apparent Specific Gravity-The weight of the oven-dry aggre-
gate divided by its absolute volume excluding the natural voids in the
2.6 Bulk Speei$c Gravity ( Oven-Dry Basib )-The weight of the
aggregate dried to constant weight in an oven at 100°C divided by its
absolute volume including the natural voids in the aggregate particles.
2.7 Bulk Specific Gravity (Saturated Surface-Dry Basis ) - The
weight of the saturated surface-dry aggregate divided by its absolute
volume including the natural voids in the aggregate particles.
2.8 Concrete -A mixture of cement, water and inert aggregates with or
2.9 Concrete Mix -A mixture of cement, water and inert aggregates
which is freshly mixed during a period of two hours from the time of addi-
tion of water to the solid ingredients.
2.10 Constant Length- The stage when the difference between two
consecutive readings taken of the dimensions of a specimen is less than a
specified value. In the case of a 15 cm specimen, this value shall be
W5 mm and for larger specimens proportionately greater.
2.11 Drying Shrinkage -‘The difference between the length of a spe&
men cut from a concrete which has been matured and subsequently
saturated, and its length when dried to constant length.
2.12 Drying Shrinkage, Initial- The difference between the length of
a specimen mouldtd and cured under specified conditions and its length
when dried to constant length.
2.13 Moisture Mo&eat -- The difference between the length of a
specimen when dried to constant length and its length when subsequently
2.14 Saturated Surf~cc-Dry Weight-The weight of aggregate whose
component pieces are saturated with water but contain no free surface
2.15 smchce Mobtwe -The moisture contained in the aggregate in
excess of that contained in the natural voids of the aggregate.
2.16 Water Cement R&O - The fatio of the weight ofwaterin a eon-
crete n&achGve of the water absorbed by aggregates to the weight of
2.17 Workability -_c property of concrete which deteimines the
amount of useful internal work necessary to produce complete compaction.
3. SAMPLING OF FRESH CONCRETE IN THE PIELD
3.1 This method specifies the procedure to be followed in the field for
obtaining representative samples of fresh concrete directly Coti the mixer
or from concrete at the time and place of depositipn.
3.2 Sample - The composite sample shall be truly representative of the
batch and shall be not less than CO2 ma in volume. It shall be composed
of a mixture of portions taken Corn d&rent points in the batch. When
continuous mixers~ are used, ” batch shall be regarded as the discharge
* from the mixture during one minute.
3.3.1 From Mixers -At least three approximately equal sample incre_
ments totalling 0.02 ms shall be taken Corn a batch during its discharge
and each sample increment shall be collected l$ passing a clean and
dry receptacle across the stream d concrete. This receptacle shall be con-
structed of non-absorbent material, preferably of metal and shall be such
that the sample retained is not segregated. A fiat surface without retain-
ing sides will not fulfil this purpose. Where three sample increments are
taken they shall be taken at about the time when one-quarter, one-halfand
three-quarters of the concrete have been discharged from the mixer and if
more than three are taken they shall be at correspondingly shorter, but
equally spaced, intervals.
3.3.2 From Concrete at k %ne and Place of Deposition-The sample
shall be taken while a batch of concrete is being, or immediately after it
has been, discharged on the site. The sample shall be collected from not
less than five weli-distributed positions, avoiding the edge of the mass
where segregation may have occurred.
3.4 Mixing the Composite Sample - The composite sample obtained
by either of the methods described above, shall be mixed on a non-absor-
bent base either with a shovel or by other-suitable implement in such a
manner as to ensure uniformity. The sample thus obtained shall be used
immediatciy for the purpose of carrying out the tats. Care ~hd be taken
to protect the sample from the weather.
36 aaeerdty op
- The following. information regwling the
a) date and time of sampling,
b) method of sampling used,
c) mix proportions (proportion of ingredienta including water,
admixtures, etc )
d) mixture Corn which delivered ( if more than one is used ),
e) the location of the sampled batch after placing, and
f) temperature and weather conditions.
4. SEGURING AND I’REPARING TBBT SPECIMENS
FROM HARDENED CONCRETE
4.1 Precautions -The clause specifies the procedure for securing and
preparing test specimens from hardened concrete in structures and
pavements. A specimen to be tested for strength shall not be removed
from the structure until the ctmcrete has become hard enough to permit
its removal without disturbing the bond between the mortar and the
coarse aggregate. Normally, the concrete shall be 14 days old before the
specimens are removed. Specimens that show abnormal defects or that
have been damaged in removal shall not be used.
4.2.1 DA%- A core drill shall be used for securing cylindrical core
specimens. For specimens taken perpendicular to the horizontal surface, a
short drill is satisfactory. For inclined holes, a diamond drill is satisfactory.
42.2 Saw - A saw shall be used for securing beam specimens from the
structure or pavement *for flexural strength tests. The saw shali have a
diamond or silicon carbide cutting edge and shall have adjustments that
permit of cutting specimens conforming to the dimensions specified
4.3 Test specimcas
4.3.1 Car S~b~iztens- A core specimen for the determination of pave-
ment thickness shall have a diameter of at least 10 cm. A core specimen
for the determination of compressive strength shall have a diameter at least
three times the maximum nominal size of the coarse aggregate used in the
concrete, and in no case shall the diameter of the specimen be less than
twice the maximum nominal size of the coarse aggregate. The length of
the specimen, when capped, shall be as nearly as practicable twice its
4.32 Beam 2+wimen- The beam specimen for the determination of
flexural strength shall normally have a cross-section of 15 x 15 cm and shall
be at least 70 cm in length.
NOTB- In manycam particularlywithprismscutfrom pavementslahr,fpe width
&zed by the sizeof the coprseaggregateand the depth by the tbtcbacuof
-Is 11199- 1959
4.4.1 CoreDrilling - A core specimen taken perpendicular to a hori-
zontal surface shall be located, when possible, with its axis perpendicular
to the bed of the concrete as originally placed. Aispecimen taken per-
pendicular to a vertical St&ace, or perpendicular to a surface with a batter,
shall be taken from near the middle of a unit of deposit.
4.4.2 Slab Removal-A sufficiently large slab shall be removed so that
the desired test specimens may be secured without the inclusion of any
concrete which has been cracked, spalled, undercut, or otherwise
4.4.3 Beam Sawing - The sawing operation shall .be so performed that
the concrete will not be weakened by shock or by heating. The sawn
surfaces shall be smooth, plane, parallel and shall be free from steps, ridges
and grooves. Care shall be taken in handling the sawn beam specimens to
avoid chipping or cracking.
4.5 Measarement of Drilled Core Specimens
4.5.1 Mean Diametcr- The mean diameter shall be determined to the
nearest millimetre from three pairs of measurements. The two measure-
ments in each pair shall be taken at right angles to each other, one pair
being taken at the middle of the core and the other pairs at the quarter
points of the depth. The mean of the six readings shall be taken as the
45.2 Height - The height of the core shall be determined by measuring
the maximum and minimum heights, which shall be reported to the
4.5.3 Position of Reinforccmmt - The positions of any remforcement shall
be determined by measuring to the nearest millimetre from the centre of
the exposed bars to the top of the core. The diameter and, if possible, the
spacing of the bars shall be recorded, and also the minimum top and
5. TESTS FOR WoRKARlLm
5.1 Slump Test
5.1.1 This method of test specifies the procedure to be adopted, either in
the laboratory or during the progress of work in the field, for determining,
by the slump test, the consistency of concrete where the nominal maximum
size of the aggregate does not exceed 38 mm.
a) Mould - The mould for the test specimen shall be in the form of
the frustum of a cone having the following internal dimensions:
The mould shall be constructed of metal ( brass or aluminiurrr
shall not be used ) of at least l-6 mm ( or 16 BG ) thickness and the
top and bottom shall be open and at right angles to the axis of the
cone. The mould shall have a smooth internal surface. It shall be
provided with suitable foot pieces and also handles to facilitate lifting
it from the moulded concrete test specimen in a vertical direction as
required by the test. A mould provided with a suitable guide
attachment may be used. A typical mould without the guide is
shown in Fig. 1.
b) Tur@ing rod - The tamping rod shall be of steel or other suitable
material, 16 mm in diameter, O-6 m long and rc urded at one end.
NOTE- To facilitate the Wing of the mould in a vertical direction, it is recom-
mended that suitable guide attachments be provided. Any rivets used in the
construction of the mould shall be countersunk flush on the inside of the cone.
Attachments should preferably be welded to the mould.
All dimensions in centimetrcs.
FIG. 1 TYPICAL MOULD FOR SLUMP TEST
- If’this test is being carried out in the field, the sample
mixed concrete shall be obtained as described in 3. In tb
case of concrete containing aggregate of maximum size more than 38 mm,
the concrete shall be wet-sieved through 14 in screen to exclude aggregati
particles bigger thaq 78 mm.
5 .l A Procedure -The internal surface of the mould shall be thoroughly
cleaned and freed from superfluous moisture and any set concrete before
commencing the test. The mould shall be placed on a smooth, horizontal,
rigid and non-absorbent surface, such as a carefully levelled metal plate,
the mould being firmly held in place while it is being filled. The niould
shall be filled in four layers, each approximately one-q6arter of the height
of the mould. Each layer shall be tamped with twenty-five strokes of the
rounded end of the tamping rod. The strokes shall be distributed in a
uniform manner over the cross-section of the mould and for the second
and subsequent layers shall penetrate in@ the underlying layer. The
bottom layer shall be tamped throughout its depth. After the top layer
has been rodded, the concrete shall be struck off level with a trowel or the
tamping rod, so that the mould is exact19 filled. Any mortar which may
have leaked out between the mould and the base plate shall be cleaned
away. The mould shall be removed from the concrete immediately by
raising it slowly and carefully in a vertical direction. This allows the
concrete to subside and the slump shall be measured immediately by
ddtermining the difference between the height of the mould and that of
the highest point of the specimen being tested. The above operations
shall be carried out at a place free from vibration or shock, and within a
ljeriod of two minutes after sampling.
5.1.5 Shm@ - The slump measured shall be recorded in terms of milli-
lnetres of subsidence of the specimen during the test. Any slump speci-
men which collapses or shears off laterally gives incorrect result and if this
occurs the test shall be repeated with another sample. If, in the repeat
test also, the specimen should shear, the slump.shall be measured and the
fact that the specimen sheared, shall be recorded.
NOTE-Some indication of the cohesiveness and workability of the mix can be
obtained, if after the slump measurement has been completed, the side of the concrete
is tapped gently with the tamping rod; a well-proportioned concrete which has an
appreciable slump will gradually slump fm’ther, but if the mix has been badly
proportioned, it is likely to fall apart.
55 Compacting Factor Test
3.2.1 This clause specifies a procedure for determining the workability
of concrete, where the nominal maximum size of the aggregate does not
exceed 38 mm. The test is designed primarily for use in the laboratory,
but if circumstances permit, it may also be used i4 the field. It is more
precise and sensitive than the slump test and is particularly useful for
concrete mixes of very low workability as are normally used &hen con-
crete ia to be compacted by vibration; such concrete may consistently f&i1
525 A##amtus- A diagram of the apparatus is shown in Fig. 2.
shall consist of the two conical hoppvs ( A and B ) mounted above a
cyrmdrical mould (C).
VIEW OF TRAP-DOOR
FIG. 2 COMPACTZNGFACTORAPPhRATus
22.214.171.124 The essential dimensions of the hoppers and mould and
distances between them shall be as shown in Table I. The hopper an
cylinder shall be of rigid construction, true to shape and smooth inside.
They shall preferably be made of cast brass or bronze, but stout sheet brass
or steel may also be considered satisfactory provided the inside surfaces
of the joints are smooth and flush. The lower ends of the hoppers shall
be closed with tightly fitting hinged trap-doors having quick release catches.
Metal plate 3 mm thick is suitable for the doors. The frame in which the
hoppers and cylinder are mounted shall be of rigid construction and shall
firmly locate them in the relative positions indicated in Table I. The
cylinder and hoppers shall be easily detachable from the frame. The
apparatus shall also include two ordinary bricklaver’s trowels, one hand
scoop about 15.2 cm long, a rod of steel or other suitable materral of l-6 cm
diameter, 61 cm long rounded at one end, and scales ( or a balance ) to
weigh up to 30 kg, to the nearest 10 g.
5.2.3 Samgling- If thii test is carried out in the field, the sample of
rreshly mixed concrete shall be obtained by the method specified under 3.
In the case of concrete containing aggregate of maximum size more than
38 mm, the concrete shall be wet;sieved through 1) in screen to exclude
aggregate particles bigger than 38 mm.
TABLE I ESSENTUL DIMENSIONS OF THE GOMPACTING FACTOR
APPARATUS FOR USE WITH AGGREGATE NOT EXCEEDING 38 mm
NOMINAL MAXIMUM SIZE
( Ckwse 126.96.36.199 )
DETAIL ( stw FIG. 2 ) DIMENSXUN
Upper hopper, A
Top internal diameter
Bottom internal diameter
Lower hopper, B
Top internal diameter 22.9
Bottom internal diameter 12-7
Internal height 22.9
Distance between bottom of upper hopper and
top of lower hopper
Distance between bottom of lower hopper and
top of cylinder
5.2.4 Prcwzeakre- ‘I%C sample of concrete TVbe tested shall be placed i
gently in the upper hopper, using the hand sccmp. The hopper shall be ’
filled level with its brim and the trap-door shall be opened so that the
concrete falls into the lower hopper.. Certain mixes have a tendency to
stick in one or both of the hoppers. If this occurs, the concrete may be
helped through by pushing the rod gently into the concrete from the top.
&ring this process, the cylinder shall be covered by the trowels. Im-
mediately after the concrete has come to rest, the cylinder shall be un-
covered, the trap-door of the lower hopper opened, and the concrete
allowed to fall into the cylinder. The excess of concrete remaining above
the level of the top of the cylinder shall then be cut off by holding a trowel
in each hand, with the plane of the blades horizontal, and nicving them
simultaneously one from each side across the top of the cylinder, at the
same time keeping them pressed on the top edge of the cylinder. The
outside of the cylinder shall then be wiped clean. The above operation
shall be carried out at a place free from vibration or shock. The ‘weight
of the concrete in the cylinder shall then be determined to the nearest
10 g. This weight shall be known as cthe weight of partially compacted
concrete ‘. The cylinder shall be refilled with concrete .from the same
sample in layers approximately 5 cm deep, the layers being heavily
rammed or preferably vibrated so as to obtain full compaction. The top
surface of the fully compacted concrete shall be carefully struck off level
with the top of the cylinder. The outside of the cylinder shall then be
Ncue- The test is sufficiently sensitive to enable differences in workability at&&
from the initial processes in the hydration of the cement to bc measured. Each tat,
therefore, should be carried out at a constant time interval after the mixing is completed
if strictly co¶ble results are to be ,obtaincd. A convenient time for releasing &
concrete from the upper hopper has been found to be 2 minutes after the completion
5.2.5 Calculation - The compacting factor is defined as the ratio of the
weight of partially compacted concrete to the weight of fully compacted
concrete. It shall normally be stated to the nearest second decimal
5.3 Flow of Cement Concrete’by the Use of the Flow Table
5.3.1 This method of test specifies the procedure for the use of the flow
table to delcrmine the fluidity of concrete, where the nominal size of the
aggregate does not exceed 38 mm.
a) Mould - The mould shall be made of a smooth metal casting, as
shown in Fig. 3 in the form of the frustum of a cone with the
following internal dimensions. A base 25 cm in diameter, upper
surface 17 cm in diameter, and height 12 cm; the base and the
top shall be open md at right angles to the axia of the cone.
The mould shall be provided with handles.
Flop @h-Flow table shall co&ormtothedaignrhowd~.
having‘s height of40 to 5Ocmandweighingnotkrrthan
Sampring- Samples for test shall be obtained by th;e nxfex+
under 3. In the case of concrete containing aggr
mum size more than 38 mm, the concrete shall be wet-siev za through Ii
in scrken to exclude aggregate particles bigger than 38 mm. They shall
be transported to the place of moulding of the specimen, and to counteract
segregation, the concrete shall be mixed with a shovel until it is.uniform
All dimensions cqntimetres.
Fro. 3 MOULD FOR FLOW TZ#T
DETAIL OF CAM
Al TM TIME OF OROP
All dimensions In centimetres.
Fxo. 4 FLOW TABLE APPARATUS
5.3.4 Procedure- Immediately preceding the test, the table top, and
inside of the motild shall be wetted and cleaned of all gritty material and
the excess water removed with a rubber squeezer. The mould, centred
on the table, shall be firmly held in place and filled in two layers, each
approximately one-half the volume of the mould. Each layer shall be
rodded with 25 strokes of a straight round metal rod 1.6 cm in dia-
meter and 61 cm long, rounded at the lower tamping end. The strokes
shall be distributed in a uniform manner over, the cross-section of the
mould and shall penetrate into the underlying layer. The bottom layer
shall be rodded throughout its depth. After the top layer has been roddd,
Is 81199- 1959
the surface of the concrete shall be struck off with a trowel so that the mould
is exactly filled. The excess concrete which has overflowed the mould shall
be removed and the area of the table outside the mould again cleaned.
The mould shall be immediately removed from the concrete by a steady
upward pull. The table shall then be raised and dropped 12.5 mm, 15
times in about 15 seconds. The diameter of the spread concrete shall
be the average of six symmetrically distributed caliper measurements read
to the nearest 5 mm.
5.3.5 Recoding -The flow of the concrete shall be recorded as the
percentage increase in diameter of the spread concrete over the base dia-
meter of the moulded concrete, calculated from the following formula:
Flow, percent =
spread diameter in cm - 25
5.4 Determination of Consistency of Concrete by Vee-Bee Consisto-
5.4.1 This clause deals with the determination of consistency of concrete
using a Vee-Bee Consistometer, which determines the time required for
transforming, by vibration, a concrete specimen in the shape of a conical
frustum into a cylinder.
5.4.2 A@aratus - The Be-Bee Consistometer ( seeFig. 5 ) consistsof:
a) A vibrator table resting upon elastic supports,
b) A metal pot,
c) A sheet metal cone, open at both ends, and
d) A standard iron rod.
188.8.131.52 The vibrator table (C) is 380 mm long and 260 mm wide
and is supported on rubber shock absorbers at a height of about 305 mm
above floor level. The table is mounted on a base (K) which rests on
three rubber feet and is equipped with an electrically operated vibrometer
mounted under it, operating on either 65 or 220 volts three phase,
50 cycles alternating current. A sheet metal cone (B) open at both ends
is placed in the metal pot (A) and the metal pot is fixed on to the
vibrator table by means of two wing-nuts (I-I). The sheet metal cone is
30 cm high and its bottom diameter is 20 cm and top diameter 10 cm. A
swivel arm holder (M) is fixed to the base and, into this is telescoped
another swivel arm (N) with funnel (D) and guide-sleeve (E). The
swivel arm can be readily detached from the vibrator table. The graduated
rod (-7) is fixed on to the swivel arm and at the end of the graduated
arm ‘8. glass disc
records the slump
of concrete after
rod is 20 mm in
(C) is screwed. The division of the scale on the rod
bf the concrete cone in centimetres and the volume
vibration of the cone in the pot. The standard iron
.diameter and 500 mm in length. The electrical
FIG. 5 VEE-BEE CO~SISTOMETER.TYPE VBR
rod is 20 mm in diameter and 500 mm in ,length. The electrical equip-
ment mounted on the base of the consistometer consists of a fixed plug
and connector for the electric supply cable, plug and socket contacts for
the detachable cable connected to the vibrometer and a control switch.
A photograph of the apparatus under operation is given in Fig. 6.
5.4.3 Procedure -A slump test as described under 5.1 shall be per-
formed’ in the sheet metal cylindrical pot of the consistometer. The glass
disc ( C ) attached to the swivel arm shall be moved and placed just on
the top of the slump cone fn the pot and before the cone is lifted up, the
position of the concrete cone shall be noted by adjusting the glass disc
attached to the swivel arm. The cone shall then be lifted up and the
slump noted on the graduated rod by lowering the glass disc on top of the
concrete cone. The electrical vibrator shah then be switched on and the
concrete shall be allowed to spread out in the pot. The vibration shah
then be continued until the whole concrete surface uniformly adheres
I’IC. 6 .'a~-BEE COSSISTOMETEW
to the glass disc as indicated in Fig. 6, and the time taken for this to be
attained shall be rioted with a stop watch. The time is recorded in seconds.
5.4.4 Resrclt -The consistency of the concrete shall be expressed in
W-degrees which tie equal to the,time in seconds recorded in 5.4.3.
* *, ‘I
, $$. .:
184.108.40.206The required slump I obtained on the basis of the consiateny
scale given in Table II. The curve in Fig. 7 indicati the relationshrp
between slumo in cm and the degrees covered by the consistency scak
given in Table II.
Fm. 7 RELATION BETWEEN SLUMP IN cm AND VEE-BEE DEOREES.
TABLE IE C6NSLSTENCY SCALE
( clwrsr 220.127.116.11. and Fig. 7 )
40 to 25-20
20 to 15-10
10 to 7-5
3 to 2-l
More fluid than 1
Particlcd of eoane aggregate in the concrete arc
adhesive, but concrete does not clot. Risk of
Concrete has the consistency of very stiff por-
ridge, forms a stiff mound when dumped,
and barely tends to shake or roll itself to form
an almost horizontal surface when
for a long time in, say, a wheel-barrow.
Concrete has the consistency of stiff porridge,
forms a mound when dumped, and shakes or
rolls itself to form a horizontal surface when
conveyed for a long time in, say, a whccl-
Concrete can be shaped into a ball between the
palms of the hands, and adhcrcs to the skin.
Concrete cannot bc rolled into a ball between
the palms of the hands, but s reads out even
though slowly and without P ccting the cohe-
sion of the constituents so that segregation
does not occur.
Concrete spreads out rapidly and segregation
6. ANALYSIS OF FRESHLY - CONCRETE
6.1 This method of analysis deals with the procedure for determinating
the proportions of the constituents of freshly mixed concrete where the
nominal size of the largest aggregate does not exceed 38 mm.
6.1 .I General Procedure - A sample of the concrete mix shall be taken
and the analysis commenced within five minutes of the time of discharge
of the concrete mix from the mixer or agitator. If this is not possible,
the sample shall be placed in an air-tight container within five minutes
of discharge and stored until the commencement of the analysis which
shall be within a period of two hours from the addition of the water to
the solid ingredients. Samples of the coarse and fine aggregates from
the consignments used for the making of the concrete shall also be taken.
Before the analysis of the concrete is carri$d out, the samples of the aggre-
gates shall be tested for specific gravity, water absorption and proportion
passing the appropriate sieves. If, .however, the aggregates are obtained
Is t 1199- 1959
from one source and the variations in the specific. gravity do not exceed
rf: O-003, for the purpose of routine control the tests on the aggregates shall
be made at agreed intervals. .
6.2 Apparatus - The following apparatus, one form of which $ shown
in Fig. 8, shall be used:
a) A semi-automatic balance capable of weighing up to 5 kg to an
accuracy of 05 g. The balance shall be provided with a
WElGHlNG IN AIR
SUISID;;;; WAlER EX7RA COUNTERPOISE FOR
-Y WEIGHING IN WITCR
. &AIN WATER TANK
E SPRAY FOR WASHING
4%PLAN OF SPIDER
MSE lb SUPPORT
NESTED SIEVES FUNNEL FOR TRANSFER
All dimensions in centimetrcs.
Fro. 8 APPARATUSFORTHE ANALYSISOF FRESH CONCRETE
counterpoise to’obtain equilibrium when an empty bucket is being
weighed in air. A second counterpoise shall be provided to
secure approximate equilibrium when an empty bucket is being
weighed whilst immersed in water. If the sample is to be weighed
in air and covered with water at the site before transport to a
laboratory for analysis, a balance capable of weighing up to 5 kg
to an accuracy of 1 g shall be available at the site.
At least eight bucket-shaped containers made of corrosion resisting
metal, each 20 cm in diameter at the ‘top and 18 cm deep, and
having sloping sides and a rounded bottom ( to prevent the trap-
ping of air when it is immersed ). The containers shall all be
of the same weight in air and each shall be clearly marked with
the necessary correction figure to allow for the difference between
its loss in weight when immersed in water and the weight of the
A tank approximately 28 cm in diameter and approximately 30 cm
deep. Thii shall have an overflow spout in such a position that
the rim of a bucket hung from the balance is completely immersed
when the tank is full. The tank shall be connected by a 6.5 mm
dia tap and flexible pipe to a subsidiary tank. This connection
shall be such that, when the tap is open and the subsidiary tank
is positioned below the main tank, the level of water in the main
tank is below the lip of a bucket hangin
on the balance. A baffle
plate, extending from the top of the tan to a position 5 cm below
the connection, shall be provided inside the main tank opposite the
connection to the subsidiary tank.
Two nesting sieves 46 cm in diameter, the upper sieve being 10 cm
deep and of IS Sieve Designation 48?, and the lower sieve being
30 cm deep and of IS Sieve Designation 15.
A funnel approximately 50 cm in diameter at the top, 15 cm dia-
meter at the bottom, and 25 cm deep.
A hose fitted with a nozzle giving a fine spray of water strong
enough to move the particles of fine aggregate over the surface of
the IS Sieve 15.
A metallic stirring rod, 1.6 cm in diameter.
6.3 Method of Taking Samples
63.1 Aggregates - Four samples of the coarse and four samples of the
fine aggregates, as used in the concrete, shall be obtained by taking one
main sample for each material and quartaing as described in *IS : 383-1952
until samples of the required size are obtained.
6.3.2 Concrctc Mix- If the test is being carried out on a concrete mix
made in the field, a sample of at least 0.02 ms obtained by the method
*Second rev~r~onin 1970.
specified under 3 shall be quartered and remixed until a representative
of sample required size is obtained.
6.39 sam@s - Samples shall be taken from each of the various sizes of
aggregates in the same nominal proportions as are used in the concrete
and such that the total weight of the samples shall be approximately
3.5 kg. The sample of concrete shall weigh approximately 4 kg if the
nominal size of coarse aggregate does not exceed 19 mm, otherwise the
sample shall weigh apprhately 8 kg and it shall be analyzed in two
parts, each weighing approximately 4 kg.
6.4 Determba don of the Speci5c Gravity of the Aggregates
6.4.1 The specific gravity of each of the aggregates shall be determined
under conditions identical with those to be applied to the analysis of the
concrete., DiEerences in the temperature of the water at the time of
making any weighings during the test shall not exceed 2°C.
6.4.2 Each sample of- the coarse and fine aggregates shall be dried in a
ventilated oven at a temperature of 100 to 110°C for 24 hours, cooled and
weighed. The weights ( in grammes ) shall be recorded as A, for the
coarse aggregate or A, for the fine aggregate.
6.4.3 Each sample shall be placed in a clean bucket [see 6.2(b) ] and
the bucket filled with water to within 25 mm of the lip. The sample shall
be stirred for one minute to remove any trapped air and the bucket hung
in the water tank from the balance. The water level in the tank shall
then be raised,steadily by raising the subsidiary tank until the water .s@rts
to run from the overfiow spout. The sample shall then be weighed in
water. During the weighing, the maximum movement of the bucket shall
be limited to 6.5 mm to avoid any inaccuracy caused by variations in its
displacement or by agitation ‘of the contents. The sample shall be left
under water for 20 minutes, stirred, roimmersed and re-weighed, and this
procedure shall be repeated until the change in weight between consecutive
weighings is less than O-5 g but in any case the period of immersion shall
not exceed 8 hours. The final weights shall be recorded as B,, for the
coarse aggregate or B, for the fine aggregate. The time required to attain
constant weight shall be recorded.
6.4.4 The specific gravities shall be calculated as follows:
Specific gravity of coarse aggregate = A
Specific gravity of fine aggregate = A*
The average specific gravity of each type of aggregate shall be
6.U The maximum the required for any of the samples to attain
instant weight shall be regarded as the time required for the absorption of
atcr by the aggregates as a whole.
6.5 6ped6c Gra&y of the Cemeatt
6.5.1 For the purposes of this test, the specific gravity ofportland cement
ihall be taken as 3.15. If other cements are used, the specific gravity shall
be determined by a recognized inert liquid method.
6.6 Sieve Analysis
6.6.1 Each of the samples used to determine the specific gravity of the
aggregates shall be used to determine the quantity of material passing each
of the appropriate sieves.
6.6.2 One sample of the coarse aggregate shall be placed on IS Sieve
480 over the IS Sieve 15 and washed for two minutes under the spray of
water, the aggregate being stirred during the washing. The material
retained on IS Sieve 480 shall then be washed into a clean bucket by
means of the funnel, stirred, immersed in water, and weighed ( weight D, ).
6.6.3 One sample of fine aggregate shall then be added to any material
retained on IS Sieve 15 and washed under~the spray of water for at least
ten minutes, continuing until the water is clear. The residue retained on
the sieve shall be washed into a clean bucket, stirred, immersed and
weighed ( weight D, ). Care shall be taken in making these tests so that no
material is lost in transferring the samples to the sieves and back to the
6.6.4 The correction factors shall be calculated as follows:
. For the coarse aggregate C, = 3
For the fine aggregate C, = --$-
NOTE -The correction factors are used to make allowance for the amount of
coarse aggregate passing IS Sieve 480 and the amount of total aggregate passing
IS Sieve 15.
6.6.5 The above procedure shall be repeated with each of the other
three samples of coarse aggregate and of fine aggregate and the average
correction factor for each type of aggregate determined.
6.6.6 The maximum time required for washing any of the samples shall
be adopted as the time required for washing the concrete on IS Sieve 15
( see6.7.9 ).
6.7 Analysis of Concrete - The sample of the concrete shall be placed
in a clean bucket and analyzed as follows.
6.7.1 The sample shall be weighed in air ( weight W).
NOTE- Thh opcratiou may be carried aut at the &e-bc$~~dc~ z
6.71 The bucket shall be filled with water to within 25 mm of the lip
and the contentsstirred thoroughly for one minute to remove any trapped
6.7.3 The sample shall be left immersed in water for a period of time
not less.than that required for absorption of water by the aggregate, as
determined in accordance with *IS : 383-1952 but in any case not longer
than 8 hours. After this period of immersion, the concrete shall again be
thoroughly stirred for one minute to remove any air expelled from the
6.7.4 The bucket shall be hung in the water tank Corn the balance with
the water level in the tank below the lip of the bucket, namely with the
subsidiarytank below the main tank and the tap open. The bucket shall
then be carefully filled with water up to the lip and the sample left to
settle for five minutes.
6.7.5 The water level in the tank shall then be raised steadily by rais-
ing the subsidiary tank, When water OV&OWS from the spout in the
main tank, the tap shall be turned olI and the sample weighed in water
( weight W). During this process,care shall be taken to avoid shaking the
sample and the maximum movement of the bucket shall be liiited to that
specifiedunder 6.42. If the water level is raised steadily, little of the water
containing fine particles of cement will spill out of the bucket. If the
water in the tank becomes discoloured, it shall be changed between
weighings to,avoid any change in its speci& gravity.
6.7.6 The concrete shall be wash.ed from the bucket on to the IS
Sieve 480 placed over IS Sieve 15 [see 6.2(d) 1, care being taken to w&
the bucket clean. The sample shall then be washed under the spray
of water for at least two minutes continuously until the coarse aggregate
is clean, the material being stirred during the washiig.
6.7.7 The clean coarse aggregate retained on the IS Sieve 480 shall
then be washed into a clean bucket by means of the funnel and spray of
water. The spray shall be used to remove any small Fartic!es from the
mesh. Unless the water at this stage is clear, the washing specified
in 6.7.6 shall be repeated before the aggregate is placed in the bucket.
6.7.8 The coarseaggregate in the bucket shall be covered with water
and stirred thoroughly for one minute. The bucket shall then be
immersed in water in the tank and the aggregate weighed as be&s-r
*Second reviniouin 1970.
6.7.9 The line aggregate rcm&ing on the IS Sieve 15 shall be washed
under the spray of water.
6.7.10 The clean line aggregate shall be washed into a clean bucket,
stirred, immersed in water and weighed as before ( weight W, ).
6.6CaIcuMa~~ofRoportions- The proportions of each constituent
in the concrete shall be calculated as follows:
The weight of coarse aggregate in the sample, W, = w,C,F,
The weight of fiue agg&te in the sample, W, = w,C,F,
The weight of cement in the sample, W, = [ w - ( w,,C, + w,C, ) ]Fo
The weight of water in the sample, W, = W - ( W,, + W, + W, )
specific gravity - 1
specific gravity - 1
specific gravity - 1
for the coarse aggregate,
for the fine aggregate,
for the cement,
W = the weight of the concrete in air,
w = the weight of the concrete in water,
W, = the weight of the coarse aggregate in water,
w,= the weight of the fine aggregate in water,
c, = the correction factor for the coarse agsegate, and
c, = the correction factor for the fine aggregate.
6.9 Water Cement Ratio -The water cement ratio by weight may be
calculated from the figures in 65 as W,l W, and shall be expressed to the
NOTE-The water/crmentrkio as dctermincd by this method includes any
water contained in the aggregate before mixing.
6.10 Report- The following information shall be reported:
4 identification mark of sample,
b) date of test,
4 weights of constituentz,
4 proportions of constituents,
4 water cement ratio, and
f 1 remarks, such as times for aggregates to attain constant weight.
7. DETERMINATION OF WlUGHT PBR CUiHC
OF FRESHLY MIXED CONCRETE
7.1 This method specifies the procedure for determining the weight per
cubic metre of freshly mixed concrete, and gives formulae for calculating
the volume of concrete per batch, the yield per bag of cement, the cement
factor, namely cement content per cubic metre, and the air content of the
NOTE -This method of calculating air content is of value particularly for air
7.2.1 Balance - The balance shall be sensitive to O-01kg.
7.2.2 Tamping Bar - The tamping bar shall be a steel bar weighing
l-8 kg, 38 cm long, and shall have a ramming face square.
7.2.3 Measure - The measure shall conform to one of the sizes specified
in Table III, according to the nominal size of the coarse aggregate in
the concrete. The measure shall have a smooth interior, and shall be
water-tight and of sufficient rigidity to retain its shape under rough usage.
The rim of the measureshall be machined to a plane surface perpendicular
to the axis of the cylinder. For convenience, the measure may be provided
18.104.22.168 Calibration of measure-The measure shall be calibrated by
determining the weight of water at room temperature required to lill it so
that no meniscus is present above the rim. Accurate filling of the
measure may be secured by the use of a glass cover plate. The capacity
of the measure in cubic metres shall then be obtained by dividing the
weight of water ( in grams ) required to fill the measure by the unit
weight of water, 1000 g/l.
TABLE I.5 DIMENSIONAL RRQB FOR
( Clause 7.2.3 )
NOMINALSIZE NOMINAL INSIDE INSlDE MINIMUMTxmxrws
OF co- CAPACITY DIAMETFZR HEwIT G3 METN,
mm cu m mm mm ----z- mm
up to 38 0.01 250 280 4 8
Over 38 oa? 350 285 5.5 5
la t 1199- 1959
7.3 Sampling - The sample of fiesn~y mixed concrete shall be obtained
in accordance with the method specified in 3 except when small batches
are made under laboratory conditions.
7.4.1 Cizm~acting - The measure shall be filled with concrete as soon
as practicable after mixing, in such a way as to produce full compaction
of the concrete with neither segregation nor excessive laitance. The
concrete shah be filled into the measure in layers approximately 5 cm deep
and each layer shall be compacted either by hand or by vibration as
described below (see 22.214.171.124 and 126.96.36.199 ). After the top layer has been
compacted, the surface of the concrete shall be struck off level with the top
of the measure.
188.8.131.52 Comwting by hand- When compacting by hand the standard
tamping bar shall be. distributed in a uniform manner over the cross-
section of the measure.
The number of strokes per layer required to produce the specified
condition will vary according to the type of concrete, but in no case shall
the concrete be subjected to less than 60 strokes per layer for the 0.01 ms
measure or 120 strokes per layer for the 0.02 ms measure.
184.108.40.206 Compacting by vibration - When compacting by vibration each
layer shall be vibrated by means of an electric or pneumatic hammer or
by means of a suitable vibrating table until the specified condition is
7.43 Tajping - The exterior surface of the cylinder shall be tapped
smartly 10 to 15 times or until no large bubbles of air appear on the sur-
face of the compacted layer.
7.4.3 Strike-Of, Cleaning and Wtighing Y After consolidation of the
concrete, the top surface shall be struck-off and and finished smoothly with
a flat cover plate using great care to leave the measure just level full. All
excess concrete shah then be cleaned from the exterior and the filled
7.5.1 Weight per Cubic Metre -The weight per cubic metre of concrete
shall be calculated by dividing the weight of fully compacted concrete in
the measure by the capacity of measure, determined in accordance
with 220.127.116.11 and shall be recorded in kg/m8.
7.5.2 Volume of Concrete ptr Batch --The volume of concrete produced
per batch shall be calculated as follows:
V = volume in cu m of concrete produced per batch,
N = number of 50 kg bags of cement per batch,
W, = total weight in kg of the tine aggregate per batch in con-
w, = total weight in kg of coarse aggregate per batch in condi-
w,= total weight in kg of mixing water added to batch, and
W = weight of concrete in kg/m’.
7.5.3 Tield per Bag of Cement - The yield shall be calculated as follows:
Y = yield of concrete per 50 kg bag of cement in ma,
V c volume of concrete produced per batch in ms, and
N- number of 50 kg bags of cement per batch.
7.5.4 Cement Factor - The cement factor shall be calculated as follows:
or N, 3 -a-
.iV,= cement factor, that is, number of 50 kg bags of cement
per cubic metre of concrete produced,
r = yield of concrete per 50 kg bags of cement in m”,
N = number of 50 kg bags of cement per batch, and
V - volume of concrete produced per batch in m3.
7.5.5 Air Content - The air content shall be calculated as follows:
orA= ~v-vA x loo
A = air content ( percentage ofvoids ) in the concrete,
7’= theoretical weight of the concrete, in kg/m3, computed
on an air-free basis,
w = weight deoncrete inkg/d,
V = volume ofeomxete produced per batch in mf and
VA -4otal absolute volume of the component ingrediienb in
the babch, in ma.
* tpercub&metredKnlldbe. outinthek~;ia*ucisuuwdto aJn8t+fOranlwhamad$
~u&&&auial coqonalt ingrcdwts 8nd prqnxtiOIn. It Is calculated &cm the
T I theorctiul weight of coacrctc in kg/n+, computed on an air-kc hrh,
WgI totalweightin kg ofthe component ingrcdicnts in the batch, and
VA w total absolute volua~e of the component ingrcdicnta in the batch in ma.
poncnts, the bulk rpccific gravity and weight should bc bawd on the
utuntod rurfaccdry condition.
For the cenun> 8 value of 915 m8y be used unlcn the actual spccifk
gravity is dttamwd by a mcognkd incrt liquid mcthod.
8. AlR CONTENT OF FBBSHLY MIXBD
WNCBBT% By THB F.BBlWURB MBTHOD
&I This method specifies the procedure for determining thi air content of
wy mixed concrete by the pressure method.
&Jon- Thi)‘metbod ia considered ad
uate for a11ordinary types of concrete4
m, except for concrcta or mortars ma e with highly porous aggrcgatca, what the
vtc correction factor connot bc detcrmlncd accwatcly by the technique found
nhdrctory fix the usual types of relatively demc natural lggrcgata.
a) MeasuringBOWL- A llanged cylindrica! bowl, preferably of steel
or hard metal not readily attacked by the cement paste, having a
&meter qua1 to 1 to 1.25 times the height. The outer rim and
upper surface of the ftange, as well as the interior surfaces of the
&owl, shall be smooth-machined surfaces. The minimum size of
the container shall be a functio? of the size of coarse aggregate
in the concrete sample.
as is specified in Table
Contamers shall be at least as la’ge
IV, depending on the size of m m
The bowl rhall be pressur&ght and sufficicn’tly rigid to limit
the expansion factor ‘D'of the apparatus assembly ( SM8,S.S )
TABLEIV MXNibUMSIZE OF CONT- coRREsPoNDlNG To
NOMINAL MAXIMUM SIZE OF A-=
Mmxmm SxzsOF NOUUtALlhRlllW
to not more than @I percent of the air content on the standpipe
indicator scale when under the normal operating pressure.
orderto reduceerrorsin sampling.
Conical Cover Asmnb& - The flanged cover, preferably of steel
or hard metal not readily attacked by the cement paste, shall
have interior surfaces inclmed not less than 30” from the hori-
zontal. The outer rim and ‘lower surlhce of the flange and the
sloping interior surface shall be pressur+tight and sufficiently rigid
to limit the expansion factor of the apparatus assembly as pre-
scribed in 8.2(a). The cover shall be fitted with a standpipe which
may be a graduated precision bore glass tube or may bc made of
metal of uniform bore with a glass water gauge attached. The
graduations for a suitable range in air content shall be in percent
and tenths of a percent as determined by the proper air pressure
calibration test. The internal diameter of the standpipe shall’ be
designed so that under the normal operating pressure the water
column will be lowered sufficiently to measure air contents up to
0.1 percent. It is suggested that approximately 25 mm lowering
of the water column should represent one percent of air. The
applied air pressure shall be indicated by a pressure gauge connect-
ed to the air chamber above the water column. The gauge shall
have a range of twice the normal working pressure with suitable
graduations. ( A pressure of 05 to 2-Okg/cm* has been used satis-
factorily. However, each container shall have to be calibrated
for a stated normal procedure. ) The cover shall be fitted with
a suitable device for venting at the top of the air chamber, an air
valve, and a petcock for bleeding off water as required. Suitable
means for clamping the cover to the bowl shall be provided to
make a pressure-tight seal without entrapping air at the joint
between the flanges of the cover and bowl. A suitable hand pump
shall be provided with the cover, either as an attachment or as
Cdibratiba @iadk-The calibration cylinder shall consist of a
cylindrical measure having an internal volume qual- to approxi-
mately 3 to 6 percent of the vohnne of the measuring bowl. A
(No. 16 BG) or
may be machined from l-6 mm brass tubing
desired ) to whi
proper diameter to provide the volume
a brassdisc6-5 mm in thickness is soldered to
form the bottom.
A Coil Spring - A coil spring or other means shall be provided for
holding the calibration cylinder in place.
Spray Tube- A tube of appropriate diametei- which may be an
integral part of the cover assembly or which may be provided
separately so constructed that when water is added to the con-
tamer, there will be a minimum of disturbance to the concrete.
A Trowel - of the ordinary bricklayer’s type.
Tamping Rod-The tamping rod shall be of steel or other suitable
material of l-6 cm dieter,. 61 cm long, and rounded at the
Mallet - A mallet with a rubber or rawhide head, weighing 250g
for containers smaller than O-01cu m capacity and 500 g or more
for larger containers.
Strike-OfBar - A strike-off bar consisting of flat straight steel
Funnel -A funnel with spout fitting into the tube described
Measure - A measure aaving a 2*5 or 5 litre capacity, asrequired
to fill .the indicator with water from the top of the concrete to
the zero mark.
83.1 Change in barometric pressure caused by change in elevation or
by changes of temperature and humidity, and rough handling under job
conditions; will affect the calibration ofprcssure type apparatus for deter-
mination of air content. The steps described under this clause are pre-
rquisites for the final calibration test to determine the operating pressureP
on the pressure gauge as described hereunder. Normally, this calibration
need be made only once ( at the time of the initial calibration ), or only
occasionally to check volume constancy of the. calibration cylinder and
measuring bowl. On the other hand, the calibration test described
in 8.3.7 must be made as frequently ax necessary,to ensurethat the proper
gauge pressure P is being us4 in tests for the air content of concrete.
Moreover, a change in elevation of more than 183 m ( 600 ft ) from the
location at which the apparatua’waa last calibrated will require calibration
in accordance with 8.3.7.
8.3.2Calibration of Ca~rvration Cllindsr -The weight of water w ( m
grammes) required to 6ll the calib tora ‘on cylinder shall be accurately
determined, using a scale sensitive to 05 g;
8.3.3 Calibration of Measuring Bowl-The waght OI water W (in
grammes ) required to fill the measuring bowl shall be determined, using a
scale sensitiveto 0.1 percent of the weight of the bowl filled with water.
A glass plate is slid carefully over the flange of the bowl in such a manner
as to ensure that the bowl is completely filled with water. ’ A thin film of
cup grease smeared on the flange of the bowl will make a water-tight joint
between the glass plate and the top of the bowl.
8.3.4 Determination of Constant R -The constant R represents the
volume ‘of the calibration cylinder expressed as percentage of the volume
of the measuring bowl. Calculate R m follows:
8.3.5 DetGrmination of Ex@nsion F&or D -The expansion factor D for
any given apparatus assemblyshall be determined by filling the apparatus
with water only ( making certain that all entrapped air has been removed
and the water level is exactly on the zero mark), and applying an air
pressureapproximately equal to the operating pressure P, determined by
the calibration test described in 8.3.7. The amount by which the water
c&mm is lowered shall be the equivalent expansion factor D for that
particular apparatus and pressure.
NOTE 1-~~thougn tnc bowl, cover and clamping mechanism of the apparatus
are so constructed that it will be reasonably m-tight, the application of
internal pressure may result in a small expansion in volume. The expansion will
not affect the test results becausk, with the procedure described in 8.4 and 8.5, the
amount of expansion is the same for the test for air in concrete as for the test for
aggregate correction factor on combined 6ne and coarse aggregates, and ia thereby
zwtomaticaily cancelled. However, it does enter into the calibration tat to
dt._zmine the air pressure to be used in testing fresh concrete and appear as the
value D in the exprcsion for the calibration factor k, equation (2) under 8.3.6.
NOTE 2 - It will ‘be sticiently accurate for .this purpose to use an approximate
value for P determined by m a preliminary calibration test as described
in 8.3.7, except that an approximate value for the calibration factor shall be used.
For thii test k E W98R which is the same as equation (2) under 8.3.6 except that the
expzkon factor D as yet unknown, is assumd to be zero.
8.3.6 D&&nation of Calibration Factor k-The calibration factor k
is the amount by which the water column shall be depressed, during the
calibration procedure to obtain the gauge pressure required to make the
graduations on the glass tube correspond directly to the percentage of air
introduced into the measuring bowl by the calibration cylinder when the
bowl is levelfull of water. calculate k as follows:
Nom-The value of k given in equation (2) is derived V?om the more general
whaz H = ratio of the volume of air in the calibration cylinder after the bowl
has been filled with water, to the volume before inundation. H decreases di htly
as the elevation above sea level increases and is about O-980 at sea level for a Lwl
20 cm daq, O-975 at 1520 m above sea level and P970 at 3 960 m above sea level.
The error mtrcduccd by neglecting these variations in the value of H will usually
be ~KBsmall ( corresponding to le4.3 than 0’05, percent air) thdt equation (2),
k = 093R + D, usually will be su5cienflv accurate. However, the value of
H shonld be checked for each design of apparatus, each 10 cm of bowl height
de&&ng the value of H by O-01.
8.3.1 Calibration Test io Determine Ojerating Pressure, P, on Pressure
Gaugc- If the rim of the calibration cylinder contains no recesses or pro-
jections, it shall be fitted with three -or more spacers equally spaced around
the circumference. Invert the cylinder and place it at the centre of the
dry bottom of the measuring bowl.
for flow of water into the
The spacers shall provide an opening
calibration cylinder when pressure is applied.
Secure the inverted cylinder against displacement and carefully lower the
conical cover. After the cover is clamped in place, carefully adjust the
apwtus assembly to a vertical position and add water at air tempera-
tnre, by means of the tube and funnel, until it rises above the zero mark
on the standpipe. Close the vent and pump air into the apparatus to the
approximate operating pressure. Incline the assembly about 30” from
the vertical and using the bottom of the bowl as a pivot, describe several
complete circles with the upper end of the standpipe, simultaneously
tapping the cdver and sides of the bowl lightly to ‘remove any entrapped
air adhering to the inner surfaces of the apparatus. Return the apparatus
to a vertical position, gradually release the pressure ( to avoid loss of air
from the calibration cylinder ) and open the vent. Bring the water level
exactly to the zero mark by bleeding water through the petcock in the top
of the conical cover. After closing the vent, apply pressure until the water
level has dropped an amount equivalent to about 0.1 to O-2 percent of air
more than the value of the calibration factor k, determined as described
in 8.3.6. To relieve local restraints, lightly tap the sides of the bowl, an?,
when the water level is exactly at the value of the calibration factor k, read
the pressure P, indicated by the gauge and record to the nearest O-01 kg/
cm%. Gradually release the pressure and open the vent to determine
whether the water level returns to the zero mark when the sides of the
bowl are tapped lightly ( failure to do SO indicates loss of air from the
calibration cylinder- or loss of water due to a leak in the assembly ). If
the water level fails to return to within 0.05 percent air of the zero mark
and no leakage beyond a few drops of water is found, some air probably
was lost from the calibration cylinder. In this case, repeat the calibration
procedure step by step from the beginning of this paragraph. If the
leakage is more than a few drops of water, tighten the leaking joint before
repeating the calibration pressure. Check the indicated pressure reading
promptly by bringing the water level exactly to zero mark, closing the
vent, and applying the pressure I’, just determined.
with a finger.
Tap the gauge lightly
When the gauge indicates the exact pressure P, the water
column should read the value of the calibration factor k, used in the first
prcssurc application within about 0.05 percent of air.
CAUTION- The apparatus asscmbl shall not be moved from the vertical
position until pressure has been applied wL ch will force water about one-third of the
way up into the calibration cylinder.
Any loss ofair from this cylinder will nullify
8.3.8 Determination of Aggregate CorrectionF&r - The aggregate correc-
tion factor shall be determined on a combined sample of fine and coarse
aggregate-s as specified in thii clause and illustrated in Fig. 9.
The weights of fme and coarse aggregates present in the volume S, of
the sample of fresh concrete whose air content is to be determined, shall,be
determined as follows:
F, = 2 x Fb ... ...
c, = ; x c, ..,. ..,. ..
9A 98 9c
*A1 = hl - IL,when bowl contains concrete as shown in this figure; when bowl cotains
only aggregate and water hl - h, = G ( aggregate correction factors), Al - G = A ( air
content, percentage by volume of concrete ).
FIG. 9 ILLUSTRATIONOF PRESSUREMETHOD OF TEST FORAIR CONTENT
F, = weight in kg of fine aggregate in concrete sample under
S = volume in ms of concrete sample ( same as volume of
measuring bowl of apparatus ),
B = volume in ma of concrete produced per batch determined
in accordance with 7,
FlJ= total weight in kg of fine aggregate in batch,
C, = weight in kg of coarse aggregate in concrete sample
under test, and
c, = total weight in kg of coarse aggregate in batch.
Mix representative samples of fine aggregate, of weight F, and coarse
awegate, of weight C,, and place in the measuring bowl filled one-third
full of water. Add the mixed aggregate, a small amount at a time, until
all the aggregate is inundated. Add each scoopful in a manner that will
entrap as little air as possible and remove accumulations of foam promptly.
Tap the sides of the bowl and lightly rod the upper layer of the aggregate
about t-en times and stir after each addition of fine aggregate to eliminate
When all of the aggregate has been placed in the bowl and inundated
for at least 5 minutes, strike off all foam and excess water and thoroughly
clean the flanges of both bowl and conical cover so that when the cover is
clamped in place, pressure-tight seal is jobtained. Complete the test as
described in 8.4.. The aggregate correction factor G is equal to ir,--h, as
determined in the tests on the aggregate.
NOTE-The aggregatecorrectionfactor VvlUvary with different aggregates. It
can be determined only by test, since apparently it is not directly related to
absorption of the particles. The test can be easily made and shall not be ignored.
Ordinarily the factor remains reasonably constant for given aggregates, but an
occasional check test is recommended.
8.4 Procedure for Determining Air Content of Concrete- Place
a representative sample of the concrete in the measuring bowl in three
equal layers, consolidating each layer by rodding the bowl. Vibration may
be substituted for rodding and by tapping the sample when the air content
of concrete placed by vibration is to be determined. When the concrete
is to be placed by rodding, consolidate each layer of concrete by about
25 strokes of the tamping rod evenly distributed over the cross-section.
Follow the rodding of each layer by tapping the sides of the bowl smartly
10 to 15 times with the mallet until the cavities left by r&ding arelevelled
out and no large bubbles of the air appear on the surface of the rodded
layer. In rodding the i!rst layer, the rod shall not forcibly strike the
bottom of the bowl. In rodding the second and final layers, only enough
force shall be used to cause the rod to penetrate the surface of the
previous layer. Slightly over6ll the howl with the third layer and, after
rodding or vibration, remove the excess concrete by sliding the str&e-oE
bar across the top flange with a sawing motion until the bowl is just
Thoroughly clean the- flanges of the bowl and of the conical cover so
that when the cover is clamped in place, a pressure-tight seal will be
obtained. Assemble the apparatus and add water over the concrete by
means of the tube until it rises to about halfway mark in the standpipe.
Incline the apparatus assembly about 30” f&m vertical end, using the
bottom of the bowl aa a pivot, dexribe several complete circles with the
upper end of the column simultaneously tapping the conical cover lightly
to remove any entrapped air bubbles above the concrete sample. Return
the apparatus assembly to its vertical position and fill the water column
slightly above the zero mark, while lightly tapping the sides of the bowl.
Foam on the surface of the water column may be removed with a syringe
or with a spray ofalcohol to provide a clear meniscus.
Bring the water level to the zero mark of the graduated tube before
closing the vent at the top of the water column ( Fig. 9A !. Apply slightly
more than the desired test pressure P ( 092 kg/cm* more ) to the concrete
by means of the small. hand pump. To relieve local restraints, tap thC
sides of the measures smartly, and when the pressure gauge indicates the
exact test pressure P (as determined iri accordance with 8.3.1 in the
calibration test ), read the water level A1arid record to the nearest division
or half division ( @IO or @05 percent air content ) on the graduated
precision bore tube or gauge glass of the standpipe ( Fig. 9B ). For
extremely harsh mixes, it may be necessary to tap the bowl vigorously
until further ‘tapping produces no change in the indicated air content.
Gradually release_the air pressure through the vent at the top of the water
column and tap the sides of the bowl lightly for about one minute.
Record the water level h,, to the nearest division or half division ( Fig. 9C ).
The apparent air content A, is equal to A1- R,. Repeat the steps specified
as above in this clause ( without adding water to re-establish the water level
at the zero mark . The two consecutive determinations of apparent air
content should check within Q2 percent of air and shall be averaged to ,
give the value A1 to be used in calculating the air content A, in accordance
8.5 Calculation - Calculate thi air content of the concrete as follows:
A air content, percentage by volume of concrete,.
A, x apparent air content; percentage by volume of concrete
( sc6 8.4 ), and
G = aggregate correction factor, percentage by volume of
concrete ( see 8.3.8 ).
9. CEMENT CONTENT oloy_T
9.1 This method of test specifies the pr.ocedure for determining the cement
content of hardened portland cement concrete except those containing
certain aggregates or admixtures which liberate soluble silica under the
conditions of the test, such as slags, diatomites and sodium silicate.
9.2.1 Hydrochloric Acid -approximately 3.3 N. Add 200 ml of hydro-
chloric acid ( sp gr 1.19 ) to 600 ml of distilled water.
.9.2.2 Sodium Hydroxide - approximately 1 N. Dissolve 20 g of hydroxide
in 200 ml of water and dilute to a volume of 500 ml.
923. Hydrojluoric Acid - 40 percent.
9.2.4 Sulphuric Acid - sp gr 1.84.
9.3 Preparation of Sample -Every precaution shall be taken to
have the sample of concrete used for analysis truly representative of the
material under consideration. Several portions weighing at least 5 kg each
shail be taken to avoid all but slight inequalities of the concrete mix.
These portions shall then be broken up, crushed in a suitable machine to
about one centimetre size and reduced to a fineness of approximately
IS Sieve 10 to IS Sieve 8 in a ball mill, disc pulveriser or by any other
suitable device. Care shall be taken that rhe finer fractions of the broken
sample, which are richer in ,cement, are not discarded or lost. After
thorough mitiing and quartering, a portion approximately 100 g shall be
taken and carefully freed, by means of a strong magnet, from particles of
metallic iron abraded from the pulveriser ball mill. The clean sample
shall then be dried at 105°C for at least 2 hours.
9.4 Procedure - Weigh into each of three 250 ml beakers, not less than
a 2 g portion of the prepared sample. Moisten with a stream of hot water,
while stirring to prevent adhesion to the beaker or the formation of lumps
in .the mass. Slowljl add 100 ml of 3.3 N hydrochloric acid and stir
thoroughly. The lumps which tend to form should be reduced with the
glass rod. After the evolution of carbon dioxide has ceased and the
reaction is apparently complete, heat gently for a few minutes and allow
the contents of thi beaker to settle. Decant through an ignited and
weighed Gooch crucible which contains a mat of short asbestos shreds,
practically insoluble in hydrochloric acid and thick enough to be opaque
to light. Once the filtration has, begun, care shall be taken so that the
mat and accumulated residue do not dry out completely until the filtration
process is complete. Regulate the suction so as to maintain a rapid rate
of dropping during the greater part of the filtration. Retain as much of
the residue in the beaker as possible. Wash by decantation twice with
hot water. Add 75 ml of 1 N
stirring and heat to about 75°C.
hot water. Transfer the residue
60 ml of hot water. ’
sodim hydroxide to the residue while
Decant as ‘before and wash twice with.
to the crucible and wash with at least
9.5 The filtrate now containsthe silica in the form of silicic acid in true
solution or in suspensionin the hydrochloric acid medium. If the aggre-
gates of the original sample are largely calcarcousor dolomitic, add 10 ml
of hydrochloric acid ( sp,gr 1.19) to the solution. Transfer to a suitable
beaker with several rinsingsof the flltqllask, Evaporate to dryness with
great care to minimize spattering, bake at not over 120°C for one hour,
moisten with hydrochloric acid ( sp gr l-19 ), evaporate and bake again
and take for filtration in 75 ml of 2 N or 3 N hydrochloric acid heated to
boiling. Filter through an ashlessfilter paper and wash the residue with
50 ml of hot 1 N hydrochloric acid and then with hot water until the
washings are free from chloride. Repeat the evaporation and filtering
processes to recover the small amounts of silica dissolved and add these!
to the first residue. Determine the silica present in the sample by trcat-
ment with hydrofluoric and sulphuric. acids in accordance with the
procedure given in Appendix A of IS : 269-1958’ .
9.6 Correction Factor -When the aggregates, used in the concrete
being analyzed, are available, a blank test shall be run on these aggregates
to determine their content of silica, soluble under the conditions of the
test (see 9.4 ). This content of the soluble silica shall then be used as a
correction factor and be subtracted from the total soluble silica found in the
concrete, the difference being due to the cement contained in the
9.7 Calculation -The percentage of cement in the sample shall be cal-
culated by dividing the percentage of silica found by the factor O-2140,
provided the silica content of the cement is not known to be different from
thisvalue. When possible, the known value shall be taken as the factor.
10. DETERMINATION OF CHANGES IN LENGTH ON
JXtIXt~ FD WETTING ( INITIAL DRYING SHRINKAGE,
10.1 Thii method of test speci6es the procedure for determining the
change in length of concrete specimensdue to changes in moisture content.
It deals with tests both on Jaboratory specimens and specimens cut from
structures or ‘units, when the maximum nominal size of the aggregate in
either does not exceed 38 mm.
10.2.1 Measuring A#fmatus - A measuring apparatus shall be used
which incorporates a micrometer gauge or a suital-It diil gauge reading
l&rend revision in Iy67. 39 .
accurately to 0905 mnL This gauge shall be rigidly mounted in a measur-
ing Game and shall have a ttcessod end which can be located upon a
6-5 mm diameter ball or other preference point cemented in the specimen
as described under X0.3. The other end of the frame shall have a similar
recea4 seating which can be located upon a second ball or referencepoint
in the specimen.
An invar steel rod of a suitable length with 6’5 mm dia-
he&al ends, or with 6.5 mm diameter steel balls mounted at
the ends shafl be used as a standard of length against which the readings
of the gauge cau be tested, thus enabling corrections to be made for any
changes in the dimensions of the apparatus between successivemeasure-
ments of a test specimen. The apparatus shall preferably be adjustable
for specimens of different lengths and invar rods shall be available in
lengths approximating to those of the specimens to be tested. Typical
fm of apparatus are shown in Fig. 10 and 11, but other suitable forms
may he used. The apparatus shown in Fig. 10 is to be prepared for large
specimens and those of higher densities, since the pressurecaused by the
weight of the specimen, which would otherwise fall on the lower reference
ball, is carried by the slotted shelf.
10.2.2 Dping Oven-The drying oven shall comply with the following
It shall have an internal volume quivalent to not less than
O-008 ma per specimen, with a minimum total volume of
It shall be reasonably air-tight and shall be provided with a fan
to keep the air circulating effectively during the drying of the
It shall be maintained at a temperature of 50 & 1%.
The humidity of the air in the oven shall be controlled at
approximately 17 percent relative humidity by meansof saturated
calcium chloride solution. Suitable dishes or trays containing
this solution shall be provided to give an exposed area of solution
not lessthan one square metre for each cubic metre volume of the
oven The dishesor trays shall contain sufficientsolid calcium chlo.
ride b show above the surface ofthe solution throughout the test.
16.3 &a+ Siue -Specimens shall be cast or cut with a length of 15 to
50 cm and a cross-sectionas near as practicable to 7.5 x 7-Scm.
103.1 cartspccirnac- Where the test iscarried out upon a specimen
y for testing, it shall, unless other curing condiuons are
be stored for the first three to seven days in moist air. During
reference points consisting of 6.5 mm diameter steel halls
or other suitable ref-ce points providing a 6-S mm diameter hemispheri-
calbearingshallbe cemented with neat rapid hardening portland cement or
other suitable cementing agent into the centre of each end of the specimen
NOTE- When apparatua ia fitbid with locknutv, u shown above, urc should he
taken that the first nut is tight beforelockingthe d out
FIG. 10 TYPICAL APPARATUS roa DRYINO SHRINKAGB AND
MOIETURB MOVEY~NT Tmm
-6-S mm DIA
DETAIL AT e
4 DETAIL ~1
FIG. 11 TYPICAL APPARATUS FOR DRYINGSHRXNKAGE AND
MOBTURE MOVEMENT Terns
after drilling or cutting a shallow depression. After fixing, the sm%&
of the balls shall be wiped clean of cement, dried, and coated with lubri-
eating grease to prevent corrosion. The specimen shall be kept moist for
at least 24 hours after tixing the balls, in order to allow the cement to
harden. At the conclusion of the period of storage in “moist air, the
specimen shall be immersed in water at a temperature of 24 to 30% until
28 days after the concrete has been made, or untli such other time as may
10.3.2 Mutursd S’ccimnrs- When the test is carried out on a specimen
cut from matured concrete or on a specimen which has not had the con-
trolled curing indicated in 10.3.1, the balls or other reference points shall be
fixed and greased as described in 10.3.1 and the specimen kept moist for at
least 24 hours after fixing the balls. The specimen shall then be immemed
in water at 24 to 30% in such a manner that one of the larger faces of
the specimen just breaks surface in the water and left so immersed for four
10.4 Procedure for Testing for Initial Drying Shrinkage or Drying
Shrinkage - Immediately after removal of the specimen from the water,
the grease shall be wiIjed from the balls and the length of the specimen
measured to an accuracy of 0.005 mm by the apparatus described in 10.2.1.
This shall be taken as the ‘ original wet measurement ‘.
NOTE -The instrument reading required is not the absolute length of the specimen
but the difference in length between the specimen and an invar rod of approximat&
the same length.
‘IYhe specilnen shall then be dried in the oven as described
under 10.2.2 at the specified temperature and humidity for at least 44
hours. The specimen shall then be removed from the oven and cooled for
at least four houq in a desiccator containing solid calcium chloride in a
saturated solution of calcium chloride. The length of the specimen shall
then be measured as described above at a temperature of 24 to 30°C.
NOTE- lf measurements are made at temperatures other than 2YC, they &odd &
reduced by PO02 percept of the dry length for each 2W above 25°C.
10.4.1 The cycle of drying, cooling and measuring shall be repeated
until constant length is attained, that is, when the difference between two
consecutive readings separated by a period,of drying of at least 4% hours,
followed by cooling for at least four hours, ,is less than 0.01 mm for a 15 cm
specimen, and proportionately greater for a larger specimen. The final
reading shall be taken as the dry measurement. During the above drying
process, further wet specimens shall not be placed in the same oven, and
there shall be a free access of air to all surfaces of the specimens.
10.43 After ,t)it: dry ‘measurement has been taken, the length of the
specimen shall be measured, adjacent, to the balls, .to the nearest 0’5 mm
and this shall be taken as the ‘ dry length ‘. The ‘ initi# drying sh&&agr ’
x6 I 1199 - 1959
or the ‘ drying shrinkage ’ shall be calculated as the difference between the
‘ or&g&l wet measurement ’ and the ‘ dry measurement’ expressed as a
percentage of the ‘ dry length ‘.
103 Determination of Moistme Movement - For the determination
of the moisture movement, the specimen shall first be tested for initial
drying shriiage or drying shrinkage as described above and the dry
measurement determined. The specimen shall then be immersed in water
at 24 to 30°C in such a manner that one of the larger faces of the specimen
just breaks surface in the water and shall be left so immersed for four days
after which the ( final wet measurement ’ shall be determined. The mois-
ture movement shall be calculated as the difference between the cdry
measurement ’ and ‘ final wet measurement ’ expressed as percentage of the
10.6 Report - The following information, shall be included in the report:
Date of starting test,
Age of specimen at beginning of test,
Size of specimen,
Initial drying shrinkage or drying shrinkage,
Moisture movement, if determined, and
Remarks, such as, time to reach constant length.
BUREAU OF INDIAN STANDARDS
Manak Bhavan, 9 Bahadur Shah Zafar Marg, NEW DELHI 110002
Telephones : 331 01 31, 331 13 75 Telegrams : Manaksanstha
( Common to all offices)
1 331331137501 31
Central : Manak Bhavan, 9 Bahadur Shah Zafar Marg,
*Eastern : 1/14 C.I.T. Scheme VII M, V. I. P. Road,
Maniktola, CALCUTTA 700054
Northern : SC0 445-446, Sector 35-C,
Southern : C. 1.1. Campus, MADRAS 600113
tWestern : Manakalaya, E9 MIDC, Marol, Andheri (East),
‘Pushpak’ Nurmohamed Shaikh Marg, Khanpur,
AH M EDABAD 360001
SPeenya Industrial Area, 1st Stage, Bangalore Tumkur Road
Gangotri Complex, 5th Floor, Bhadbhada Road, T. T. Nagar,
Plot No. 82/83, Lewis Road, BHUBANESHWAR 751002
63/5, Ward No. 29, R. G. Barua Road, 6th Byelane,
5856C I. N. Gupta Marg ( Nampally Station Road),
Rl4 Yudhister Marg, C Scheme, JAIPUR 302005
117/418 B Sarvodaya Nagar, KANPUR 208005
Patliputra Industrial Estate, PATNA 800013
T.C. No. 14/1421, University P.O., Palayam
lnspecflon Oftce (With Sale Point) :
Pushpanjali, 1st Floor, 205-A West High Court Road,
Shankar Nagar Square, NAGPUR 440010
Institution of Engineers ( India ) Building, 1332 Shivaji Nagar,
*Sales Oftke In Calcutta is at 5 Chowringhee Approach, P.O. Prlncep
Street, Calcutta 700072
Wales Office In Bombay Is at Novelty Chambers, Grant Road,
*Sales Ofnce in Bangalore Is at Unity Building, Nararimharaja Square
41 24 42
38 49 55
38 49 56
5 36 27
3 31 77
6 98 32
21 68 76
21 82 92
2 51 71
27 68 00
22 36 71
Prlntrd at Slmco Prlntlno Prow. Oolhi. India
_~ ~_._-._ ___“__~..___ __.-. --...